In larger casting, they can be up to a millimetre (0.040 in) in diameter.To prevent gas porosity the material may be melted in a vacuum, in an environment of low-solubility gases, such as argon or carbon dioxide, or under a flux that prevents contact with the air. To minimize gas solubility the superheat temperatures can be kept low. Turbulence from pouring the liquid metal into the mould can introduce gases, so the moulds are often streamlined to minimize such turbulence. Other methods include vacuum degassing, gas flushing, or precipitation. Precipitation involves reacting the gas with another element to form a compound that will form a dross that floats to the top. For instance, oxygen can be removed from copper by adding phosphorus; aluminium or silicon can be added to steel to remove oxygen. A third source consists of reactions of the molten metal with grease or other residues in the mould. Hydrogen is produced by the reaction of the metal with humidity or residual moisture in the mould. Drying the mould can eliminate this source of hydrogen formation.Gas porosity can sometimes be difficult to distinguish from micro shrinkage because microshrinkage cavities can contain gases as well. In general, microporosities will form if the casting is not properly risered or if a material with a wide solidification range is cast. If neither of these are the case then most likely the porosity is due to gas formation. Tiny gas bubbles are called porosities, but larger gas bubbles are called blowholes or blisters.
Such defects can be caused by air entrained in the melt, steam or smoke from the casting sand, or other gasses from the melt or mould. (Vacuum holes caused by metal shrinkage (see above) may also be loosely referred to as blowholes). Proper foundry practices, including melt preparation and mould design, can reduce the occurrence of these defects. Because they are often surrounded by a skin of sound metal, blowholes may be difficult to detect, requiring harmonic, ultrasonic, magnetic, or X-ray (e.g., industrial CT scanning) analysis. Pouring metal defects
Pouring metal defects include misruns, cold shuts, and inclusions. A misrun occurs when the liquid metal does not completely fill the mould cavity, leaving an unfilled portion. Cold shuts occur when two fronts of liquid metal do not fuse properly in the mould cavity, leaving a weak spot. Both are caused by either a lack of fluidity in the molten metal or cross-sections that are too narrow. The fluidity can be increased by changing the chemical composition of the metal or by increasing the pouring temperature. Another possible cause is back pressure from improperly vented mould cavities.Misruns and cold shuts are closely related and both involve the material freezing before it completely fills the mould cavity. These types of defects are serious because the area surrounding the defect is significantly weaker than intended. The castability and viscosity of the material can be important factors with these problems.